evaluation of the performance of shotcrete in structural ... of the performance of shotcrete in...
Post on 05-Apr-2018
Embed Size (px)
Evaluation of the performance of shotcrete in structural rehabilitation
Marta Oliveira dos Santos
AFA, Air Force Academy, Portugal
IST, Technical University of Lisbon, Portugal
Abstract: Shotcrete is a continuous method of projecting concrete at high velocity, without the help of any formwork. This technique is being used, with great success, in the rehabilitation of reinforced concrete structures. The main advantages of using shotcrete, when compared with the use of regular concrete, are the flexibility, the compaction, the ability of adhesion to various materials and the remission of the formwork. The objective of this study is to characterize shotcrete in some of its most important parameters, named its mechanical and durability properties, which was achieved by running laboratory tests: compression tests, pull-off tests (bond strength), permeable porosity tests, accelerated carbonation tests and chloride ion penetration tests. Test panels with 1.90 x 1.90 m
2 were projected with two different dry mixtures
of shotcrete, one with 350 kg/m3 of cement and another with 450 kg/m
3. The panels were placed
vertically and horizontally, to allow their projection in the horizontal and in the vertical (upwards direction), respectively. The rehabilitation works of a water reservoir slab where shotcrete was applied are also described. KEYWORDS: shotcrete, dry-mix, compression resistance, carbonation, ion chloride penetration, bond strength.
1. INTRODUCTION Shotcrete can be applied in almost all the cases in which conventional concrete is used. The choice of its use depends on the balance of many factors such as convenience, cost and the type of work. It is quite common to use this technique in new structures construction such as vaults, tunnels, canals, reservoirs and sewers. Another major area of application of shotcrete is the repair and strengthening of structures such as bridges, sewer systems, dams, walls, swimming pools, among others. The sprayed concrete can be reinforced with fibers and is applied for conventional or refractory purposes. The fibers can be of steel or synthetic, like glass fibers and polypropylene, and its addition in concrete increases its resistance to bending, shear and impact. Water reducers are commonly used in the wet-mix in order to improve workability without increasing the ratio a/c. Retarding admixtures are also used in the wet method and enable the extension of time working for the same mixture. Chemical-set accelerators may be implemented in both the dry-mix and the wet-mix processes (ACI 506R-05, 2005; Ryan, 1973). These increase the initial stiffness, which increases the productivity of the process by reducing the number of layers and may even increase the early strength of concrete. The disadvantage of using this type of additives is that some of them decrease the ultimate strength of concrete, so the dosage rates should be kept to a minimum. Pozzolanic admixtures, like silica fume and fly ash, can be used in shotcrete. These materials provide a better workability to concrete, making it easier to pump in case of wet-mix process. In addition to that, they may provide more resistant to penetration of sulfates and to alkali-silica reactivity. Shotcrete can achieve results quite competitive when compared with conventional concrete, in terms of cost, since it dispenses the assembly of formwork; in terms of mobility and accessibility, since the associated equipment is portable, it allows reaching inaccessible areas, and in terms of compatibility, since shotcrete has the ability to adhere to various materials such as concrete, steel and wood (Ryan, 1973). The main disadvantage comes from the rebound of coarse aggregates in shotcrete, which is affected by various factors like the speed of projection, the caudal projection, the distance and angle of impact, the thickness to be applied and, especially in dry-mix process, the operator's technical abilities (Ryan, 1973).
Shotcrete can be applied using two different methods: the dry-mix process and the wet-mix process. The main difference between these methods is that, in dry-mix process, the water is only added to the mixture in the nozzle, immediately prior to the application of shotcrete, while in the wet-mix method water is mixed with the other components in the beginning. In terms of mechanical properties of shotcrete, specifically the bond strength and the compressive strength, it can be noticed that this material should develop a minimum value of 0.7 MPa for the tensile bond strength and for the compressive strength values between 40 to 50 MPa for the dry-mix process, and values between 30 to 50 MPa for the wet-mix (ACI 506R-05, 2005). In the case of bond strength the substrate treatment is the determining factor in adherent ability between itself and the shotcrete, while the compressive strength depends mainly on the aggregates/cement (ag/cm) and water/cement (w/cm) ratios. The smaller the a/c ratio is, the more compact the concrete will be and, consequently, the greater its strength will be. In the case of dry-mix shotcrete, several authors indicate that its possible to achieve very low values for the a/c ratio, such as 0:35 to 0:50 (Cnovs, 1984) or 0:30 to 0:40 (ACI 506R-05, 2005), while in the wet-mix process, the a/c ratio must be higher to give the necessary plasticity to concrete for their pumping. The volume of permeable voids is an important factor in the durability of shotcrete, making it more or less susceptible to phenomena like carbonation and chloride diffusion. Values between 14 and 17% are acceptable for permeable shotcrete void volume (ACI 506R-05, 2005).
2. EXPERIMENTAL CAMPAIGN
2.1. Composition of shotcrete mixtures In the composition of shotcrete it was used Portland cement type CEM I 42.5 R, washed sand with two different dimensions and a gravel with 6.35 mm for maximum dimension. Applying the Faury method, two compositions of shotcrete were calculated. The results for each one of them appear below, in Table 1.
Table 1 Shotcrete composition for the test panels.
Cement kg/m3 350 450
Sand 02 kg/m3 632 614
Sand 04 kg/m3 300 269
Gravel kg/m3 678 642
Water l/m3 123 158
a/cm - 0.35 0.35
ag/cm - 4.60 3.39
2.2. Execution of the test panels Before the shotcrete application, test panels, with 1.90 x 1.90 m
2, were built. First, these panels
were reinforced with an electro-welded steel frame and were filled with a concrete class C30/37 until they reach a thickness of about 8 cm, obtaining thus the concrete substrate. Besides that, it was also placed a geotextile over the surface of the panels, which was regularly wet, to hydrate the concrete. Of the five panels produced, two were placed horizontally (Figure 2a), so that the projection was made from the upwards direction and the remaining panels were placed vertically (Figure 1b).
Figure 1 Painel direction: (a) horizontal and (b) vertical.
72 days after the substrate concrete application, two types of substrate treatment were performed: water washing (hydromilling) and chipping with jackhammers, as its shown in Table 2. After that, all panels were filled with shotcrete layers until a thickness of 7 cm was reached. Finally the concrete hydration was done with the help of a geotextile cloth which was periodically wet with water. It should be noted that this activity was performed following the parameters listed in NP EN 14487-2.
Table 2 Test panels identification.
Cement composition (kg/m
Chipping H 450
During the projection works, it was observed that the concrete was not being applied with the correct pressure. Only after the work was complete it was found that due to a clog in the oil filter, the machine did not create enough pressure in the chamber. The problem was resolved by changing the filter; however the test panels were already finished at the time.
2.3. Shotcrete characterization testing methods
2.3.1. Pull-off test The pull-off test aims to assess the ability of adhesion between the coating layer, whether it is a mortar or a concrete, and the substrate. This test consists in the application of a tensile force perpendicular to the surface (Figure 2) and is regulated by the NP EN 14488-4. With a drill a circular part is cut up to the base material, in order to define exactly the measuring surface. Then a metallic disc is glued to the lining of reinforcement with a resin glue. (Austin, et al., 1995; ASTM D7234, 2005).
Figure 2 Schematic representation of the of pull-off test phases.
Three types of scenarios may occur while executing a pull-off test and they are described in detail in Table 3.
Tabel 3 Classification and description of the pull-off scenarios.
Typology Failure mode Description
A Adhesive Rupture through the interface
between the shotcrete and support
B Cohesive in the
reinforcement concrete Rupture in the shotcrete
C Cohesive in the
substrate concrete Rupture in the subtstrate
2.3.2. Compressive strength test
The compressive strength test consists of a gradual application of load at a constant speed, on the whole contact surface of the specimen, until the ultimate load is achieved. All tests were performed according to NP EN 12390-3. To determine the compressive strength of shotcrete two types of study were performed in parallel: one on cores extracted from test panels, according to NP EN 12504-1, and another